- By
**Anita** - Follow User

- 562 Views
- Uploaded on

Download Presentation
## HIGH SPEED FSW MODELING

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

### HIGH SPEED FSW MODELING

Vanderbilt University: Welding and Automation Laboratory: Nashville, TN

Dr. Reginald Crawford

Thomas S. Bloodworth III

Paul A. Fleming

David H. Lammlein

Tracie Prater

Dr. George E. Cook

Dr. Alvin M. Strauss

Dr. D. Mitch Wilkes

Los Alamos National Laboratory: Los Alamos, NM.

Dr. Daniel A. Hartman

OVERVIEW

- Introduction
- Experimental Method/Setup
- Mechanical Models
- Simulation
- Results
- Conclusions
- Current and Future Work

INTRODUCTION

- Current uses of FSW:
- Aerospace (Spirit, Boeing, Airbus)
- Railway (Hitachi Rail)
- Shipbuilding/marine (Naval vessels)
- Construction industries and others (Audi)
- Moving to lighter materials (e.g. Aluminum)
- Conflict: 3-D contours difficult with heavy duty machine tool type equipment

INTRODUCTION

- Ideally see widely applicable industrial robots equipped for FSW
- Benefits:
- lower costs
- energy efficient
- 3-D contours etc.
- Problem: High axial forces required to FSW (1-12+ kN or 225-2700+ lbs), difficult to maintain even using robust robots especially at large distances from the base unit
- Possible solution: Utilize increased rotational speed/decreased axial force relationship to aid in developing a larger operational envelope for high speed FSW

EXPERIMENTAL METHOD

- Purpose: Examine axial forces during high speed friction stir welding with respect to mechanistic defect development due to process parameter variation
- Two Mechanical Models
- Smooth Tool Pin (Preliminary)
- Threaded Tool Pin (More Comprehensive)
- Parameters (Variables)
- Rotational Speed (RS)
- Travel Speed (TS)

EXPERIMENTAL METHOD

- Model solved with CFD package FLUENT for steady state solutions
- Force simulated for the three spatial dimensions as well as torque
- Experimental force and torque data recorded using a Kistler dynamometer (RCD) Type 9124 B

EXPERIMENTAL SETUP

- VU FSW Test Bed: Milwaukee #2K Universal Milling Machine utilizing a Kearney and Treker Heavy Duty Vertical Head Attachment modified to accommodate high spindle speeds.
- Samples- AA 6061-T6: 76.2 x 457.2 x 6.35 mm (3 x 18 x ¼”)
- Rotational Speeds: 1000-5000 RPM
- Travel Speeds: 290 - 1600 mm min-1 (11.4 in min-1 – 63 in min-1)

V-Belt and

Pulley System

Air/Oil Lube System

Vertical Head

Air/Oil

Delivery Lines

Dynamometer

Axial Position Monitor

Tool

Sample

Backing Plate

VUWAL Test Bed

EXPERIMENTAL SETUP

- The tool was set up for a constant 2o lead angle
- Fine adjustments in plunge depth have been noted to create significant changes in force data as well as excess flash buildup
- Therefore, significant care and effort was put forth to ensure constant plunge depth of 3.683 mm (.145”)
- Shoulder plunge constant: .1016 mm (.0040 in)

SMOOTH PIN MODEL

- Heat transfer to the support anvil ignored
- Tool pin and sample finite element mesh consists of
- 22497 tetrahedron brick elements
- 5152 nodes
- Tool properties were for H-13 tool steel (e.g. density, specific heat, and thermal conductivity)
- Assumed to rotate counter-clockwise at RS (LH)
- 12.7 mm shank included to account for heat conduction from the tool/sample interface

SMOOTH PIN MODEL

Tool Rotational Direction

Flow Domain Outlet

- Tool assumed to rotate with uniform and constant angular velocity, RS.
- Weld material is assumed incoming from the left upon the rotating tool
- Origin of the system is interface at the center of the pin bottom and the sample
- Sample given metallurgic properties (i.e. AA6061-T6)

Flow Domain Inlet

Tool Shank

Sample Top

Sample Side

Tool Shoulder

Flow Direction

Sample Bottom

Weld Plate

Smooth tool pin

THREADED PIN MODEL

- 2nd Model incorporates the #10-24 TPI Left-Handed thread
- Incorporates the threaded tool pin, and heat sinks on the shank
- Heat conductivity to the anvil is included
- Identical metallurgic properties given to pin and sample as the smooth pin model
- Anvil properties - Cold rolled steel

THREADED PIN MODEL

- Tool mesh:
- 37051 tetrahedron brick elements
- 8324 nodes
- Sample mesh:
- 92018 tetrahedron brick elements
- 20672 nodes
- Anvil mesh:
- 42200 quadrilateral brick elements
- 24024 nodes
- Density of mesh increases with respect to the pin/weld material interface

FLUENT: ASSIGNMENTS AND ASSUMPTIONS

- Goal: Compare the two models’ steady state welding conditions with experimentally determined data
- Flow inlet given constant flow rate (TS)
- Zero heat flux condition
- bounding regions transfer no heat to/from the weld
- No-slip (sticking) condition
- all rotational velocity of the tool is transmitted to the weld material at the interface
- Temperature was simulated for both mechanical models

TEMPERATURE SIMULATION

- Temperature was simulated using the heat generation model developed by Schmidt H. et al. The contact stress is approximated as,

= 241 MPa, AA 6061-T6

- The total heat generation approximated as:

w0 = rotational speed of tool

Rs = shoulder radius

Rp = pin radius

h = height of the pin

- Solutions were generally of the order 104 W/mm3

TEMPERATURE CONTINUED

- Subsequent simulations to determine welding temperature were run and input into FLUENT via user defined C code
- Method inherently ignores transient state including initial plunge and TS ramp up; creates an isothermal model
- The Visco Plastic model used to determine flow stress and viscosity ( and m respectively)
- Weld plate region: visco-plastic material

VISCO-PLASTIC MODEL

- Seidel, Ulysse, Colegrove et al. implemented VP model very successfully at relatively low wp
- RS: 500 rpm
- TS: 120 mm min-1 (5.11 in min-1)
- High wp implies:
- Increase RS or
- Decrease TS
- Geometries use VP model with 10-13 fold parametric increase accurately

VISCO-PLASTIC MODEL

- The VP model determines stress as,

Constants and Variables

Z = Zener-Hollomon parameter

R = Universal gas constant

T = absolute temperature (K)

= effective strain-rate

a, A, n, and Q = material constants

- Viscosity is approximated as,

- The model is therefore a function of Temperature, T, and the effective strain-rate,

AXIAL FORCE SIMULATION

- Smooth pin model: a reference pressure was included to compensate for the lack of an anvil (open domain)
- Pref = FZ/Ap
- Threaded pin model includes anvil:
- no reference pressure is necessary (closed domain)

1137 mm min-1

1353 mm min-1

1607 mm min-1

3000 RPM, 289.56 mm min-1

2250 RPM, 289.56 mm min-1

1500 RPM

2250 RPM

3000 RPM

3750 RPM

Surface deformation

PROCEDURE- Experimental sequence performed by holding the TS constant and increasing the RS incrementally until the weld matrix set was either complete or excessive surface defect occurred
- Samples etched for inspection for worm-holes (low wp)

RESULTS

- Both models correlate well with experimental results
- Greater convergence at high wp
- Increased RS/decreased Fz relationship continues for high speed FSW

TS=685.9mm min-1 (27 in min-1)

TS=1137.92mm min-1 (44.8 in min-1)

RESULTS

- Fz increases as expected for increasing TS when RS constant
- Limit to the RS increase/Fz decrease not met
- This relationship is key to widespread implementation of FSW
- It is also well known that welding torque decreases for increased RS
- Mz<50 N @ RS>1500 rpm (Mz<13 lbs)

Fz vs. TS for RS = 1500 rpm

Mz vs. RS for TS = 685.9 mm min-1

CONCLUSIONS

- The smooth pin model correlated better than the threaded pin model for all simulations
- However, threaded model more accurately represents the experimental setup
- anvil, heat sinks, pin profile
- Increase in RS led to greater correlation in both models with respect to the experimental data
- Barrier to high speed FSW is overheating and subsequent surface flash

Dynamometer

Motor

Feedback

Linear Position

Encoders

Schematic of most recent VUWAL data collection instrumentation

FUTURE WORK- Possible solutions to high speed FSW problems
- Non-rotating, floating, or differentially rotating shoulder
- Implementing force control scheme
- Other control possibilities include acoustic signal analysis, temperature analysis, etc.
- Currently implementing three axes of linear position control as well as thermal imagery as a possible segway to future control schemes
- Latest rotational speeds exceeding 6500 RPM
- Latest travel speeds exceed 3810 mm min-1 (150 in min-1)
- Repeat using butt weld configuration and investigate unconventional weld defects through various stress testing

ACKNOWLEDGEMENTS

- Completion of this was made possible through support provided by an American Welding Society and a NASA GSRP Fellowship grant
- Additional funding was provided by the NASA Space Grant Consortium of Tennessee and Los Alamos Natl. Laboratory. Los Alamos, NM
- Dr. Author C. Nunes of the NASA Marshall Space Flight Center provided valuable expertise and guidance through private communication which contributed to the completion of this work

REFERENCES

- Cook G.E., Crawford R., Clark D.E. and Strauss A.M.: ‘Robotic Friction Stir Welding’. Industrial Robot 2004 31 (1) 55-63.
- Mills K.C.: Recommended Values of Thermo-physical Properties for Commercial Alloys. Cambridge, UK 2002.
- Schmidt H., Hattel J. and Wert J.: ‘An Analytical Model for the Heat Generation in Friction Stir Welding’. Modeling and Simulation in Materials Science and Engineering 2004 12 143–57.
- Crawford R: Parametric Quantification of Friction Stir Welding. M.S. Thesis, Vanderbilt University, Nashville, Tennessee 2005.
- Seidel T. U. and Reynolds A.P.: ‘Two-dimensional friction stir welding process model based on fluid mechanics’.Science and Technology of Welding & Joining 2003 8 (3), 175-83.

REFERENCES

- Colgrove P.A. and Shercliff H.R.: ‘Development of Trivex friction stir welding tool Part 2 – three-dimensional flow modelling’. Science and Technology of Welding & Joining 2004, 9(3) 352-61.
- Ulysse P.: ’Three-dimensional modeling of the friction stir-welding process’ International Journal of Machine Tools & Manufacture 2002 42 1549–57.
- Sheppard T. and Jackson A.: ‘Constitutive equations for high flow stress of aluminum alloys’ Material Science and Technology 1997 13 203-9.
- FLUENT, Fluid Dynamic Analysis Package, version 6.122 Fluid Dynamics International, Evanston, IL.
- Talia G.E. and Chaudhuri J.: A Combined Experimental and Analytical modeling Approach to Understanding Friction Stir Welding. Department of Mechanical Engineering Presentation, Wichita State University, Wichita, KS 2004.

Download Presentation

Connecting to Server..